#------------------------------------------------------------------------------
#$Date: 2021-05-26 10:36:43 +0300 (Wed, 26 May 2021) $
#$Revision: 265502 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/28/1562875.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1562875
loop_
_publ_author_name
'Kangas, Michael J.'
'Schmitt, Devin C.'
'Sakai, Akito'
'Nakatsuji, Satoru'
'Chan, Julia Y.'
_publ_section_title
;
 Structure and physical properties of single crystal PrCr2Al20 and
 CeM2Al20 (M=V, Cr): A comparison of compounds adopting the CeCr2Al20
 structure type
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              274
_journal_page_last               281
_journal_paper_doi               10.1016/j.jssc.2012.06.035
_journal_volume                  196
_journal_year                    2012
_chemical_formula_moiety         'Al20 Cr2 Yb'
_chemical_formula_sum            'Al20 Cr2 Yb'
_chemical_formula_weight         816.64
_space_group_IT_number           227
_space_group_name_Hall           '-F 4vw 2vw 3'
_space_group_name_H-M_alt        'F d -3 m :2'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   14.473(13)
_cell_length_b                   14.473(13)
_cell_length_c                   14.473(13)
_cell_measurement_reflns_used    394
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.034
_cell_measurement_theta_min      0.998
_cell_volume                     3032(5)
_computing_cell_refinement
'Denzo and scalepack (Otwinski & Minor, 1997)'
_computing_data_collection       'Collect (Nonius 1999)'
_computing_data_reduction
'Denzo and scalepack (Otwinski & Minor, 1997)'
_computing_molecular_graphics    'Crystal maker'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'Direct Methods, SIR97'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Nonius Kappa CCD'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0409
_diffrn_reflns_av_sigmaI/netI    0.0432
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            701
_diffrn_reflns_theta_full        29.85
_diffrn_reflns_theta_max         29.85
_diffrn_reflns_theta_min         2.44
_exptl_absorpt_coefficient_mu    8.666
_exptl_absorpt_correction_T_max  0.7810
_exptl_absorpt_correction_T_min  0.7810
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL scalepack (Otwinski & Minor, 1997)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       fragment
_exptl_crystal_F_000             3024
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.830
_refine_diff_density_min         -1.248
_refine_diff_density_rms         0.180
_refine_ls_extinction_coef       0.00011(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.363
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         248
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.363
_refine_ls_R_factor_all          0.0366
_refine_ls_R_factor_gt           0.0299
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0501
_refine_ls_wR_factor_ref         0.0521
_reflns_number_gt                224
_reflns_number_total             248
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            JSSC-2012-196-274.cif
_cod_data_source_block           YbCr2Al20
_cod_original_sg_symbol_Hall     '-F 4vw 2vw'
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               1562875
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x, z, y'
'y+1/4, -z, x+1/4'
'y+1/4, x+1/4, -z'
'x+1/4, -z, y+1/4'
'-z, y+1/4, x+1/4'
'z+1/4, x+1/4, -y'
'y+1/4, z+1/4, -x'
'z+1/4, y+1/4, -x'
'-z+1/4, x, -y+1/4'
'x+1/4, z+1/4, -y'
'y, -z+1/4, -x+1/4'
'x, -z+1/4, -y+1/4'
'-z+1/4, y, -x+1/4'
'x+1/4, -y, z+1/4'
'y+1/4, -x, z+1/4'
'x, -y+1/4, -z+1/4'
'y, -x+1/4, -z+1/4'
'-y, -z, -x'
'-x+1/4, -y+1/4, z'
'-y, -x, -z'
'-z, -x, -y'
'-z, -y, -x'
'z, -x+1/4, -y+1/4'
'x, y+1/2, z+1/2'
'x, z+1/2, y+1/2'
'y+1/4, -z+1/2, x+3/4'
'y+1/4, x+3/4, -z+1/2'
'x+1/4, -z+1/2, y+3/4'
'-z, y+3/4, x+3/4'
'z+1/4, x+3/4, -y+1/2'
'y+1/4, z+3/4, -x+1/2'
'z+1/4, y+3/4, -x+1/2'
'-z+1/4, x+1/2, -y+3/4'
'x+1/4, z+3/4, -y+1/2'
'y, -z+3/4, -x+3/4'
'x, -z+3/4, -y+3/4'
'-z+1/4, y+1/2, -x+3/4'
'x+1/4, -y+1/2, z+3/4'
'y+1/4, -x+1/2, z+3/4'
'x, -y+3/4, -z+3/4'
'y, -x+3/4, -z+3/4'
'-y, -z+1/2, -x+1/2'
'-x+1/4, -y+3/4, z+1/2'
'-y, -x+1/2, -z+1/2'
'-z, -x+1/2, -y+1/2'
'-z, -y+1/2, -x+1/2'
'z, -x+3/4, -y+3/4'
'x+1/2, y, z+1/2'
'x+1/2, z, y+1/2'
'y+3/4, -z, x+3/4'
'y+3/4, x+1/4, -z+1/2'
'x+3/4, -z, y+3/4'
'-z+1/2, y+1/4, x+3/4'
'z+3/4, x+1/4, -y+1/2'
'y+3/4, z+1/4, -x+1/2'
'z+3/4, y+1/4, -x+1/2'
'-z+3/4, x, -y+3/4'
'x+3/4, z+1/4, -y+1/2'
'y+1/2, -z+1/4, -x+3/4'
'x+1/2, -z+1/4, -y+3/4'
'-z+3/4, y, -x+3/4'
'x+3/4, -y, z+3/4'
'y+3/4, -x, z+3/4'
'x+1/2, -y+1/4, -z+3/4'
'y+1/2, -x+1/4, -z+3/4'
'-y+1/2, -z, -x+1/2'
'-x+3/4, -y+1/4, z+1/2'
'-y+1/2, -x, -z+1/2'
'-z+1/2, -x, -y+1/2'
'-z+1/2, -y, -x+1/2'
'z+1/2, -x+1/4, -y+3/4'
'x+1/2, y+1/2, z'
'x+1/2, z+1/2, y'
'y+3/4, -z+1/2, x+1/4'
'y+3/4, x+3/4, -z'
'x+3/4, -z+1/2, y+1/4'
'-z+1/2, y+3/4, x+1/4'
'z+3/4, x+3/4, -y'
'y+3/4, z+3/4, -x'
'z+3/4, y+3/4, -x'
'-z+3/4, x+1/2, -y+1/4'
'x+3/4, z+3/4, -y'
'y+1/2, -z+3/4, -x+1/4'
'x+1/2, -z+3/4, -y+1/4'
'-z+3/4, y+1/2, -x+1/4'
'x+3/4, -y+1/2, z+1/4'
'y+3/4, -x+1/2, z+1/4'
'x+1/2, -y+3/4, -z+1/4'
'y+1/2, -x+3/4, -z+1/4'
'-y+1/2, -z+1/2, -x'
'-x+3/4, -y+3/4, z'
'-y+1/2, -x+1/2, -z'
'-z+1/2, -x+1/2, -y'
'-z+1/2, -y+1/2, -x'
'z+1/2, -x+3/4, -y+1/4'
'-x, -y, -z'
'-x, -z, -y'
'-y-1/4, z, -x-1/4'
'-y-1/4, -x-1/4, z'
'-x-1/4, z, -y-1/4'
'z, -y-1/4, -x-1/4'
'-z-1/4, -x-1/4, y'
'-y-1/4, -z-1/4, x'
'-z-1/4, -y-1/4, x'
'z-1/4, -x, y-1/4'
'-x-1/4, -z-1/4, y'
'-y, z-1/4, x-1/4'
'-x, z-1/4, y-1/4'
'z-1/4, -y, x-1/4'
'-x-1/4, y, -z-1/4'
'-y-1/4, x, -z-1/4'
'-x, y-1/4, z-1/4'
'-y, x-1/4, z-1/4'
'y, z, x'
'x-1/4, y-1/4, -z'
'y, x, z'
'z, x, y'
'z, y, x'
'-z, x-1/4, y-1/4'
'-x, -y+1/2, -z+1/2'
'-x, -z+1/2, -y+1/2'
'-y-1/4, z+1/2, -x+1/4'
'-y-1/4, -x+1/4, z+1/2'
'-x-1/4, z+1/2, -y+1/4'
'z, -y+1/4, -x+1/4'
'-z-1/4, -x+1/4, y+1/2'
'-y-1/4, -z+1/4, x+1/2'
'-z-1/4, -y+1/4, x+1/2'
'z-1/4, -x+1/2, y+1/4'
'-x-1/4, -z+1/4, y+1/2'
'-y, z+1/4, x+1/4'
'-x, z+1/4, y+1/4'
'z-1/4, -y+1/2, x+1/4'
'-x-1/4, y+1/2, -z+1/4'
'-y-1/4, x+1/2, -z+1/4'
'-x, y+1/4, z+1/4'
'-y, x+1/4, z+1/4'
'y, z+1/2, x+1/2'
'x-1/4, y+1/4, -z+1/2'
'y, x+1/2, z+1/2'
'z, x+1/2, y+1/2'
'z, y+1/2, x+1/2'
'-z, x+1/4, y+1/4'
'-x+1/2, -y, -z+1/2'
'-x+1/2, -z, -y+1/2'
'-y+1/4, z, -x+1/4'
'-y+1/4, -x-1/4, z+1/2'
'-x+1/4, z, -y+1/4'
'z+1/2, -y-1/4, -x+1/4'
'-z+1/4, -x-1/4, y+1/2'
'-y+1/4, -z-1/4, x+1/2'
'-z+1/4, -y-1/4, x+1/2'
'z+1/4, -x, y+1/4'
'-x+1/4, -z-1/4, y+1/2'
'-y+1/2, z-1/4, x+1/4'
'-x+1/2, z-1/4, y+1/4'
'z+1/4, -y, x+1/4'
'-x+1/4, y, -z+1/4'
'-y+1/4, x, -z+1/4'
'-x+1/2, y-1/4, z+1/4'
'-y+1/2, x-1/4, z+1/4'
'y+1/2, z, x+1/2'
'x+1/4, y-1/4, -z+1/2'
'y+1/2, x, z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, y, x+1/2'
'-z+1/2, x-1/4, y+1/4'
'-x+1/2, -y+1/2, -z'
'-x+1/2, -z+1/2, -y'
'-y+1/4, z+1/2, -x-1/4'
'-y+1/4, -x+1/4, z'
'-x+1/4, z+1/2, -y-1/4'
'z+1/2, -y+1/4, -x-1/4'
'-z+1/4, -x+1/4, y'
'-y+1/4, -z+1/4, x'
'-z+1/4, -y+1/4, x'
'z+1/4, -x+1/2, y-1/4'
'-x+1/4, -z+1/4, y'
'-y+1/2, z+1/4, x-1/4'
'-x+1/2, z+1/4, y-1/4'
'z+1/4, -y+1/2, x-1/4'
'-x+1/4, y+1/2, -z-1/4'
'-y+1/4, x+1/2, -z-1/4'
'-x+1/2, y+1/4, z-1/4'
'-y+1/2, x+1/4, z-1/4'
'y+1/2, z+1/2, x'
'x+1/4, y+1/4, -z'
'y+1/2, x+1/2, z'
'z+1/2, x+1/2, y'
'z+1/2, y+1/2, x'
'-z+1/2, x+1/4, y-1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Yb1 Yb 0.1250 0.1250 0.1250 0.0137(3) Uani 1 24 d S . .
Cr1 Cr 0.5000 0.5000 0.5000 0.0074(4) Uani 1 12 d S . .
Al1 Al 0.48692(13) 0.1250 0.1250 0.0087(4) Uani 1 4 d S . .
Al2 Al 0.05900(6) 0.05900(6) 0.32515(9) 0.0113(3) Uani 1 2 d S . .
Al3 Al 0.0000 0.0000 0.0000 0.0182(8) Uani 1 12 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Yb Yb -0.3850 5.5486 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al3 Yb1 Al3 109.5 6 4
Al3 Yb1 Al3 109.5 6 3
Al3 Yb1 Al3 109.5 4 3
Al3 Yb1 Al3 109.5 6 .
Al3 Yb1 Al3 109.5 4 .
Al3 Yb1 Al3 109.5 3 .
Al3 Yb1 Al2 58.451(7) 6 147
Al3 Yb1 Al2 58.451(7) 4 147
Al3 Yb1 Al2 100.27(2) 3 147
Al3 Yb1 Al2 150.27(2) . 147
Al3 Yb1 Al2 100.27(2) 6 126
Al3 Yb1 Al2 58.451(7) 4 126
Al3 Yb1 Al2 58.451(7) 3 126
Al3 Yb1 Al2 150.27(2) . 126
Al2 Yb1 Al2 50.88(4) 147 126
Al3 Yb1 Al2 58.451(7) 6 172
Al3 Yb1 Al2 100.27(2) 4 172
Al3 Yb1 Al2 58.451(7) 3 172
Al3 Yb1 Al2 150.27(2) . 172
Al2 Yb1 Al2 50.88(4) 147 172
Al2 Yb1 Al2 50.88(4) 126 172
Al3 Yb1 Al2 58.450(7) 6 .
Al3 Yb1 Al2 150.27(2) 4 .
Al3 Yb1 Al2 58.450(7) 3 .
Al3 Yb1 Al2 100.26(2) . .
Al2 Yb1 Al2 95.127(9) 147 .
Al2 Yb1 Al2 95.127(9) 126 .
Al2 Yb1 Al2 50.01(5) 172 .
Al3 Yb1 Al2 58.450(7) 6 2
Al3 Yb1 Al2 58.450(7) 4 2
Al3 Yb1 Al2 150.27(2) 3 2
Al3 Yb1 Al2 100.26(2) . 2
Al2 Yb1 Al2 50.01(5) 147 2
Al2 Yb1 Al2 95.127(9) 126 2
Al2 Yb1 Al2 95.127(9) 172 2
Al2 Yb1 Al2 116.898(14) . 2
Al3 Yb1 Al2 150.27(2) 6 118
Al3 Yb1 Al2 58.450(7) 4 118
Al3 Yb1 Al2 58.450(7) 3 118
Al3 Yb1 Al2 100.26(2) . 118
Al2 Yb1 Al2 95.127(9) 147 118
Al2 Yb1 Al2 50.01(5) 126 118
Al2 Yb1 Al2 95.127(9) 172 118
Al2 Yb1 Al2 116.898(14) . 118
Al2 Yb1 Al2 116.898(14) 2 118
Al3 Yb1 Al2 150.26(2) 6 176
Al3 Yb1 Al2 100.26(2) 4 176
Al3 Yb1 Al2 58.449(7) 3 176
Al3 Yb1 Al2 58.448(7) . 176
Al2 Yb1 Al2 145.22(3) 147 176
Al2 Yb1 Al2 95.125(9) 126 176
Al2 Yb1 Al2 116.898(14) 172 176
Al2 Yb1 Al2 95.123(9) . 176
Al2 Yb1 Al2 145.22(3) 2 176
Al2 Yb1 Al2 50.87(4) 118 176
Al3 Yb1 Al2 150.26(2) 6 159
Al3 Yb1 Al2 58.449(7) 4 159
Al3 Yb1 Al2 100.26(2) 3 159
Al3 Yb1 Al2 58.448(7) . 159
Al2 Yb1 Al2 116.898(14) 147 159
Al2 Yb1 Al2 95.125(9) 126 159
Al2 Yb1 Al2 145.22(3) 172 159
Al2 Yb1 Al2 145.22(3) . 159
Al2 Yb1 Al2 95.123(9) 2 159
Al2 Yb1 Al2 50.87(4) 118 159
Al2 Yb1 Al2 50.87(4) 176 159
Al1 Cr1 Al1 66.84(7) 154_565 8_556
Al1 Cr1 Al1 180.0 154_565 58
Al1 Cr1 Al1 113.16(7) 8_556 58
Al1 Cr1 Al1 113.16(7) 154_565 104_665
Al1 Cr1 Al1 180.0 8_556 104_665
Al1 Cr1 Al1 66.84(7) 58 104_665
Al1 Cr1 Al1 66.84(7) 154_565 121_655
Al1 Cr1 Al1 66.84(7) 8_556 121_655
Al1 Cr1 Al1 113.16(7) 58 121_655
Al1 Cr1 Al1 113.16(7) 104_665 121_655
Al1 Cr1 Al1 113.16(7) 154_565 25
Al1 Cr1 Al1 113.16(7) 8_556 25
Al1 Cr1 Al1 66.84(7) 58 25
Al1 Cr1 Al1 66.84(7) 104_665 25
Al1 Cr1 Al1 180.0 121_655 25
Al1 Cr1 Al2 63.63(2) 154_565 142
Al1 Cr1 Al2 63.63(2) 8_556 142
Al1 Cr1 Al2 116.37(2) 58 142
Al1 Cr1 Al2 116.37(2) 104_665 142
Al1 Cr1 Al2 119.74(5) 121_655 142
Al1 Cr1 Al2 60.26(5) 25 142
Al1 Cr1 Al2 63.63(2) 154_565 73
Al1 Cr1 Al2 119.74(5) 8_556 73
Al1 Cr1 Al2 116.37(2) 58 73
Al1 Cr1 Al2 60.26(5) 104_665 73
Al1 Cr1 Al2 63.63(2) 121_655 73
Al1 Cr1 Al2 116.37(2) 25 73
Al2 Cr1 Al2 117.190(15) 142 73
Al1 Cr1 Al2 116.37(2) 154_565 169_556
Al1 Cr1 Al2 60.26(5) 8_556 169_556
Al1 Cr1 Al2 63.63(2) 58 169_556
Al1 Cr1 Al2 119.74(5) 104_665 169_556
Al1 Cr1 Al2 116.37(2) 121_655 169_556
Al1 Cr1 Al2 63.63(2) 25 169_556
Al2 Cr1 Al2 62.810(15) 142 169_556
Al2 Cr1 Al2 180.0 73 169_556
Al1 Cr1 Al2 119.74(5) 154_565 50
Al1 Cr1 Al2 63.63(2) 8_556 50
Al1 Cr1 Al2 60.26(5) 58 50
Al1 Cr1 Al2 116.37(2) 104_665 50
Al1 Cr1 Al2 63.63(2) 121_655 50
Al1 Cr1 Al2 116.37(2) 25 50
Al2 Cr1 Al2 117.190(15) 142 50
Al2 Cr1 Al2 117.190(15) 73 50
Al2 Cr1 Al2 62.810(15) 169_556 50
Al1 Cr1 Al2 60.26(5) 154_565 146_565
Al1 Cr1 Al2 116.37(2) 8_556 146_565
Al1 Cr1 Al2 119.74(5) 58 146_565
Al1 Cr1 Al2 63.63(2) 104_665 146_565
Al1 Cr1 Al2 116.37(2) 121_655 146_565
Al1 Cr1 Al2 63.63(2) 25 146_565
Al2 Cr1 Al2 62.810(15) 142 146_565
Al2 Cr1 Al2 62.810(15) 73 146_565
Al2 Cr1 Al2 117.190(15) 169_556 146_565
Al2 Cr1 Al2 180.00(4) 50 146_565
Al1 Cr1 Al2 116.37(2) 154_565 46_655
Al1 Cr1 Al2 116.37(2) 8_556 46_655
Al1 Cr1 Al2 63.63(2) 58 46_655
Al1 Cr1 Al2 63.63(2) 104_665 46_655
Al1 Cr1 Al2 60.26(5) 121_655 46_655
Al1 Cr1 Al2 119.74(5) 25 46_655
Al2 Cr1 Al2 180.0 142 46_655
Al2 Cr1 Al2 62.810(15) 73 46_655
Al2 Cr1 Al2 117.190(15) 169_556 46_655
Al2 Cr1 Al2 62.810(15) 50 46_655
Al2 Cr1 Al2 117.190(15) 146_565 46_655
Cr1 Al1 Cr1 171.54(8) 30_644 25_544
Cr1 Al1 Al2 64.25(4) 30_644 126
Cr1 Al1 Al2 124.21(7) 25_544 126
Cr1 Al1 Al2 124.22(7) 30_644 118
Cr1 Al1 Al2 64.24(4) 25_544 118
Al2 Al1 Al2 59.97(7) 126 118
Cr1 Al1 Al1 56.58(3) 30_644 100_665
Cr1 Al1 Al1 116.52(3) 25_544 100_665
Al2 Al1 Al1 111.26(3) 126 100_665
Al2 Al1 Al1 149.582(5) 118 100_665
Cr1 Al1 Al1 56.58(3) 30_644 99_656
Cr1 Al1 Al1 116.52(3) 25_544 99_656
Al2 Al1 Al1 111.26(3) 126 99_656
Al2 Al1 Al1 149.582(5) 118 99_656
Al1 Al1 Al1 60.0 100_665 99_656
Cr1 Al1 Al1 116.52(3) 30_644 128_654
Cr1 Al1 Al1 56.58(3) 25_544 128_654
Al2 Al1 Al1 149.582(5) 126 128_654
Al2 Al1 Al1 111.26(3) 118 128_654
Al1 Al1 Al1 60.0 100_665 128_654
Al1 Al1 Al1 90.0 99_656 128_654
Cr1 Al1 Al1 116.52(3) 30_644 82_545
Cr1 Al1 Al1 56.58(3) 25_544 82_545
Al2 Al1 Al1 149.582(5) 126 82_545
Al2 Al1 Al1 111.26(3) 118 82_545
Al1 Al1 Al1 90.0 100_665 82_545
Al1 Al1 Al1 60.0 99_656 82_545
Al1 Al1 Al1 60.0 128_654 82_545
Cr1 Al1 Al2 62.28(3) 30_644 185
Cr1 Al1 Al2 119.98(3) 25_544 185
Al2 Al1 Al2 63.60(3) 126 185
Al2 Al1 Al2 92.23(5) 118 185
Al1 Al1 Al2 60.14(4) 100_665 185
Al1 Al1 Al2 110.21(3) 99_656 185
Al1 Al1 Al2 89.19(4) 128_654 185
Al1 Al1 Al2 146.01(4) 82_545 185
Cr1 Al1 Al2 62.28(3) 30_644 156
Cr1 Al1 Al2 119.98(3) 25_544 156
Al2 Al1 Al2 63.60(3) 126 156
Al2 Al1 Al2 92.23(5) 118 156
Al1 Al1 Al2 110.21(3) 100_665 156
Al1 Al1 Al2 60.14(4) 99_656 156
Al1 Al1 Al2 146.01(4) 128_654 156
Al1 Al1 Al2 89.19(4) 82_545 156
Al2 Al1 Al2 114.98(6) 185 156
Cr1 Al1 Al2 119.98(3) 30_644 145
Cr1 Al1 Al2 62.28(3) 25_544 145
Al2 Al1 Al2 92.23(5) 126 145
Al2 Al1 Al2 63.60(3) 118 145
Al1 Al1 Al2 146.01(4) 100_665 145
Al1 Al1 Al2 89.19(4) 99_656 145
Al1 Al1 Al2 110.20(3) 128_654 145
Al1 Al1 Al2 60.14(4) 82_545 145
Al2 Al1 Al2 152.91(8) 185 145
Al2 Al1 Al2 57.86(5) 156 145
Cr1 Al1 Al2 119.98(3) 30_644 170
Cr1 Al1 Al2 62.28(3) 25_544 170
Al2 Al1 Al2 92.23(5) 126 170
Al2 Al1 Al2 63.60(3) 118 170
Al1 Al1 Al2 89.19(4) 100_665 170
Al1 Al1 Al2 146.01(4) 99_656 170
Al1 Al1 Al2 60.14(4) 128_654 170
Al1 Al1 Al2 110.20(3) 82_545 170
Al2 Al1 Al2 57.86(5) 185 170
Al2 Al1 Al2 152.91(8) 156 170
Al2 Al1 Al2 114.97(6) 145 170
Al2 Al2 Al1 60.02(3) 172 176
Al2 Al2 Al2 120.0 172 12
Al1 Al2 Al2 149.581(5) 176 12
Al2 Al2 Al2 120.0 172 10
Al1 Al2 Al2 149.581(5) 176 10
Al2 Al2 Al2 60.0 12 10
Al2 Al2 Cr1 115.51(3) 172 73_445
Al1 Al2 Cr1 55.49(3) 176 73_445
Al2 Al2 Cr1 115.01(2) 12 73_445
Al2 Al2 Cr1 115.01(2) 10 73_445
Al2 Al2 Al1 146.01(4) 172 130
Al1 Al2 Al1 101.19(4) 176 130
Al2 Al2 Al1 90.81(4) 12 130
Al2 Al2 Al1 61.07(3) 10 130
Cr1 Al2 Al1 54.09(3) 73_445 130
Al2 Al2 Al1 146.01(4) 172 145
Al1 Al2 Al1 101.20(4) 176 145
Al2 Al2 Al1 61.07(3) 12 145
Al2 Al2 Al1 90.81(4) 10 145
Cr1 Al2 Al1 54.09(3) 73_445 145
Al1 Al2 Al1 59.72(8) 130 145
Al2 Al2 Al2 90.43(4) 172 70
Al1 Al2 Al2 60.45(4) 176 70
Al2 Al2 Al2 89.57(4) 12 70
Al2 Al2 Al2 144.24(5) 10 70
Cr1 Al2 Al2 58.595(8) 73_445 70
Al1 Al2 Al2 104.81(4) 130 70
Al1 Al2 Al2 55.95(4) 145 70
Al2 Al2 Al2 90.43(4) 172 122
Al1 Al2 Al2 60.45(4) 176 122
Al2 Al2 Al2 144.24(5) 12 122
Al2 Al2 Al2 89.57(4) 10 122
Cr1 Al2 Al2 58.595(8) 73_445 122
Al1 Al2 Al2 55.95(4) 130 122
Al1 Al2 Al2 104.81(4) 145 122
Al2 Al2 Al2 109.96(5) 70 122
Al2 Al2 Yb1 65.00(2) 172 .
Al1 Al2 Yb1 125.01(5) 176 .
Al2 Al2 Yb1 64.565(19) 12 .
Al2 Al2 Yb1 64.565(19) 10 .
Cr1 Al2 Yb1 179.49(5) 73_445 .
Al1 Al2 Yb1 125.51(4) 130 .
Al1 Al2 Yb1 125.51(4) 145 .
Al2 Al2 Yb1 121.546(6) 70 .
Al2 Al2 Yb1 121.546(6) 122 .
Yb1 Al3 Yb1 180.0 97 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Yb1 Al3 3.133(3) 6
Yb1 Al3 3.133(3) 4
Yb1 Al3 3.133(3) 3
Yb1 Al3 3.134(3) .
Yb1 Al2 3.196(3) 147
Yb1 Al2 3.196(3) 126
Yb1 Al2 3.196(3) 172
Yb1 Al2 3.196(3) .
Yb1 Al2 3.196(3) 2
Yb1 Al2 3.196(3) 118
Yb1 Al2 3.196(3) 176
Yb1 Al2 3.196(3) 159
Cr1 Al1 2.565(2) 154_565
Cr1 Al1 2.565(2) 8_556
Cr1 Al1 2.565(2) 58
Cr1 Al1 2.565(2) 104_665
Cr1 Al1 2.566(2) 121_655
Cr1 Al1 2.566(2) 25
Cr1 Al2 2.804(3) 142
Cr1 Al2 2.804(3) 73
Cr1 Al2 2.804(3) 169_556
Cr1 Al2 2.804(3) 50
Cr1 Al2 2.804(3) 146_565
Cr1 Al2 2.804(3) 46_655
Al1 Cr1 2.565(2) 30_644
Al1 Cr1 2.566(2) 25_544
Al1 Al2 2.703(3) 126
Al1 Al2 2.703(3) 118
Al1 Al1 2.826(4) 100_665
Al1 Al1 2.826(4) 99_656
Al1 Al1 2.826(4) 128_654
Al1 Al1 2.826(4) 82_545
Al1 Al2 2.838(3) 185
Al1 Al2 2.838(3) 156
Al1 Al2 2.838(3) 145
Al1 Al2 2.838(3) 170
Al2 Al2 2.702(4) 172
Al2 Al1 2.703(3) 176
Al2 Al2 2.746(3) 12
Al2 Al2 2.746(3) 10
Al2 Cr1 2.804(3) 73_445
Al2 Al1 2.838(3) 130
Al2 Al1 2.838(3) 145
Al2 Al2 2.922(3) 70
Al2 Al2 2.922(3) 122
Al3 Yb1 3.134(3) 97
